- Amorphous brazing foil
filler metal(FM) alloys that can be produced as amorphous brazing foils (ABF) are eutecticcompositions formed by transition metals such as nickel, iron, copper, etc., in combination with metalloids, such as silicon, boronand phosphorus. In conventional crystalline state, all these materials are inherently brittle and cannot be produced in continuous forms such as foil, wire, etc. Therefore, they were available only as powders, pastes, or their derivates. On the other hand, the very presence of metalloids at or near the eutectic concentration promotes the rapid solidification (RS) conversion of such alloys into a ductile amorphous foil.
The production of
amorphous alloys requires a manufacturing technology that operates on the basis of the necessary cooling rates, which is known as rapid solidification, or melt spinningtechnology. Amorphous structures are characterized by the absence of a crystal lattice or a long range order. With this random, spatially uniform arrangement of the constituent atoms, their structure is similar to that of liquids.The nature of this production process is the reason why amorphous alloys are offered only in the form of thin, ductile metal foils. Subsequently, tapes, parts and premorms can be made by e.g. slitting, cutting, stamping and etching.
Amorphous brazing foils are compositionally much more uniform even after crystallization, they melt over a narrow temperature range under transient heating. This is a consequence of the shorter distances over which atoms of different elements have to diffuse in order to form a uniform liquid phase. The resulting instant melting and their superior flow characteristic is only one of the important features of ABFs. The absence of the residual organic solvent bases evident in powder paste/tapes correspondingly eliminates soot formation and furnace fouling. The low level of gaseous impurities in ABFs, due to the specific characteristics of its production technology, is an attractive feature for vacuum furnace brazing.
ABFs are available as strip with a width from 0.5mm to 125mm and a thickness from 20µm to 50µm. Preforms can be easily produced by using punch and die, cutting/slitting, photochemical etching, and other methods. It is simple to use foils and preforms at automatic production and assembling steps. The use of foils and preforms reduces waste and enhances manufacturing efficiency. Drying and evaporation operations, which are required with powder/paste and tape forms, are not necessary. The optimal amount of
brazingmaterial can be easily applied to the component and, in just one heating cycle, ABFs create uniform braze joints of outstanding quality.
* [http://www.Vitrobraze.com VACUUMSCHMELZE (D)] Producer of amorphous brazing foils
* [http://www.wesgometals.com WESGO (USA)] Producer of amorphous brazing foils
* [http://www.hitachi-metals.co.jp/e/index.html HITACHI (JP)] Producer of amorphous brazing foils
* [http://www.brazingfoil.com BRAZING FOIL.COM (USA)] Producer of amorphous brazing foils
Wikimedia Foundation. 2010.
Look at other dictionaries:
Brazing — This article is about the metal joining process. For the cooking technique, see braising. Brazing practice Brazing is a metal joining process whereby a filler metal is heated above and distributed between two or more close fitting parts by… … Wikipedia
Filler metal — A filler metal is a metal added in the making of a joint through welding, brazing, or soldering. Four types of filler metals exist mdash;covered electrodes, bare electrode wire or rod, tubular electrode wire and welding fluxes. Sometimes… … Wikipedia
ABF — is a three letter acronym that may refer to: * ABF Freight System, Inc. * American Bar Foundation * Applications By Forms, a component of CA OpenIngres * Arbetarnas bildningsförbund, Swedish for the Workers Educational Association * Army… … Wikipedia
NanoFoil — is the trademarked name for a reactive multi layer foil material, sometimes referred to as a pyrotechnic initiator of two mutually reactive metals, aluminium and nickel, sputtered to form thin layers to create a laminated foil. On initiation by a … Wikipedia